A WIDE-BAND, POLARIZATION-INSENSITIVE
AND WIDE-ANGLE TERAHERTZ METAMATERIAL
C. Gu, S. Qu, Z. Pei, H. Zhou, and J. Wang
College of Science
Air Force Engineering University Xi’an 710051, China
Institute of Telecommunication and Engineering Air Force Engineering University
Xi’an 710077, China Z. Xu
Electronic Materials Research Laboratory Key Laboratory of Ministry of Education Xi’an Jiaotong University
Xi’an 710049, China P. Bai and W. Peng
Synthetic Electronic Information System Research Department Air Force Engineering University
Xi’an 710051, China
Abstract—In this paper, a band, polarization-insensitive, wide-angle terahertz metamaterial absorber is presented. Simulated results show that the absorber can achieve polarization-insensitive, wide-angle absorptions in a wide band from 4.15 to 4.85 THz. The retrieved impedance shows that the impedance of the absorber could be tuned, in the absorption band, to match approximatively that of free space on one side and to mismatch on the other side, rendering both the reflectance and transmission minimal and thus the corresponding absorbance maximal. The simulated absorbances under three different
Metamaterials (MMs) are artificially designed media composed of subwavelength-engineered units, exhibiting unique electromagnetic properties that are unattainable with natural materials. With MMs, peculiar phenomena such as negative refraction [1, 2] can be obtained. MMs are ideal for the investigation of novel physical phenomena and promising for future applications. Potential applications such as superlensing with a flat slab , cloaking , miniature antennas , and many other novel functional devices have been proposed and studied.
Recently, the design of resonant metamaterial absorbers (MAs) with near-unity absorbance has been proposed at microwave and THz bands [6, 7]. Later, several efforts have been made on MAs to achieve polarization-insensitive absorption [8, 9], wide-angle absorption [10–12] and multiband absorption [13, 14]. These MAs display great absorption capability. However, they are strongly dependent on electromagnetic resonances, thus their bandwidth is rather narrow, no more than 10% relative to the center frequency. This narrowband feature of these MAs limits their potential applications in many functional devices such as microbolometers , thermal detectors , and solar cells [17, 18]. In this work, a terahertz MA, which is difficult to be achieved by naturally occurring materials, is proposed. The MA is wide-band, polarization-insensitive and wide-angle. Simulated results show that the absorber can achieve polarization-insensitive, wide-angle absorptions in a wide band from 4.15 to 4.85 THz.
2. DESIGN AND SIMULATION
(a) (b) (c)
Figure 1. The front structure (a), the back ring (b) and the unit cell (c). Geometrical dimensions are: b1 = 9.75µm, w1 = 0.25µm, b2 = 12.1µm,w2 = 1µm, b3= 9µm and p= 18µm.
to that of short wire pairs , resulting from antiparallel currents in parallel metallic segments. The electromagnetic response can be tuned by changing the geometry parameters of the front structure, back ring and spacing between them. To maximize the absorption of the MA, both the transmission and reflection should be minimized. Thus, the impedance of the absorber should be tuned to match approximatively that of free space on one side and mismatch on the other side in the absorption band. This can lead to a minimal reflectance, a minimal transmission and hence a maximal absorbance. Because of the coupling between the back ring and front patch as well as the front ring, there may exist two resonances. The wide-band property of the MA could be realized by making different resonances overlap. The polarization-insensitive and wide-angle property could be realized by improving the symmetry of the unit cell . Because of this, square patches and rings, which have good symmetry, are adopted.
Computer simulation of the MA was performed using the commercial finite difference time domain solver (CST Microwave Studio 2008). The program simulated a single unit cell as shown in Fig. 1(c) with proper boundary conditions, i.e., perfect electric boundary (XZ-plane) and perfect magnetic boundary (Y Z-plane). The other two boundaries were set to be waveports. By such boundary settings, an infinite MA slab was simulated with plane wave impinging on it. Using CST, the structure of the MA was optimized under normal incidence. The substrate (εr = 4.9, loss tangent tanδ = 0.025) is 5µm thick. By the simulation, the frequency-dependentS parameters, S11, S21, S22 and S12, can be obtained. The frequency-dependent
absorbances under three different front structures were calculated by A(ω) = 1− |S11|2− |S21|2, as shown in Fig. 2.
is only the ring, there is a 87.3% absorption peak at 4.10 THz, which is due to the resonance resulting from the coupling between the back ring and the front ring. The absorption bandwidth, in which the absorbance is greater than 50%, is 0.49 THz. These results indicate that the wide-band property could be realized by making different resonances overlap. Meanwhile, when the front structure includes both the patch and the ring, the low-frequency resonance at 4.28 THz arises mainly from the coupling between the back ring and the front ring, and the high-frequency resonance at 4.68 THz is mainly resulted from the coupling between the back ring and the front patch.
Real parts of the complex wave impedance (Z) can be retrieved from the simulated S parameters for two different transmission directions , as shown in Fig. 3. When the wave propagates along +Z, the average value of real parts of the impedance in 4.15–4.85 THz is 0.8, and it matches approximately the impedance of free space on the front side. When the wave propagates along−Z, the average value of real parts of the impedance in 4.15–4.85 THz is 0.04, which does not match the impedance of free space. These results suggest that
Figure 2. Simulated absorbances of the MA for three different front structures.
Figure 4. Simulated absorbance values under different polarization angles for TE (a) and TM (b) waves. Simulated absorbance values under different angles of incidence for TE (c) and TM (d) waves. the impedance of the absorber could be tuned to match approximately that of free space on one side while to mismatch on the other side in the absorption band. This can lead to minimal reflectance and transmission, and thus to maximal absorbance.
It is also interesting to explore the power loss in the MA since it can provide information about how and where the absorption happens. Fig. 5 compares the absorbances under three different loss conditions. When the substrate is lossy and the metal is copper, the 90% absorption bandwidth is 0.70 THz and an averaged 91.4% energy is absorbed. When the substrate is loss-free and the metal is copper, the 90% absorption bandwidth is still 0.70 THz, and an averaged 91.4% energy is consumed, too. When the substrate is lossy and the metal is perfect electric conductor (PEC), only an averaged 72.6% energy is consumed in the 60% absorption band. The simulated absorbances under three different loss conditions suggest that high absorbance is mainly due to the metallic absorption (Ohmic loss). The dielectric loss of the substrate is minor compared with the metallic absorption. This is different from previous studies on frequency selective surfaces (FSSs) where metallic absorption was relatively insignificant in comparison with dielectric loss of the substrate .
The distribution of the surface current in the MA was also calculated. In Fig. 6, a vector plot of the surface current density in the MA at 4.5 THz is presented. From Fig. 6(a), there are obvious anti-parallel currents between the patch and the ring in the front structure.
Figure 6. The distribution of the surface current density in the MA at 4.5 THz. (a) The front view; (b) the 3-D view.
From Fig. 6(b), comparatively small anti-parallel currents between the front structure and the back ring can be seen. It can be concluded that the magnetic response is supplied by the front structure which is also the chief supplier of electric response.
1. Veselago, V. G., “The electrodynamics of substances with simultaneously negative values of ε and µ,” Sov. Phys. Usp., Vol. 10, 509, 1968.
2. Shelby, R. A., D. R. Smith, and S. Schultz, “Experimental verification of a negative index of refraction,” Science, Vol. 292, No. 5514, 77–79, 2001.
3. Smith, D. R., D. Schurig, M. Rosenbluth, S. Schultz, S. A. Ramakrishna, and J. B. Pendry, “Limitations on subdiffraction imaging with a negative refractive index slab,”
Appl. Phys. Lett., Vol. 82, No. 10, 1506–1508, 2003.
4. Schurig, D., J. J. Mock, B. J. Justice, S. A. Cummer, J. B. Pendry, A. F. Starr, and D. R. Smith, “Metamaterial electromagnetic cloak at microwave frequencies,”Science, Vol. 314, No. 5801, 977– 980, 2006.
5. Enoch, S., G. Tayeb, P. Sabouroux, N. Gu´erin, and P. Vincent, “A metamaterial for directive emission,”Phys. Rev. Lett., Vol. 89, No. 21, 213902, 2002.
6. Landy, N. I., S. Sajuyigbe, J. J. Mock, D. R. Smith, and W. J. Padilla, “Perfect metamaterial absorber,”Phys. Rev. Lett., Vol. 100, 207402, 2008.
7. Tao, H., N. I. Landy, C. M. Bingham, X. Zhan, R. D. Averitt, and W. J. Padilla, “A metamaterial absorber for the terahertz regime: Design, fabrication and characterization,” Opt. Express, Vol. 16, No. 10, 7181–7188, 2008.
8. Landy, N. I., C. M. Bingham, T. Tyler, N. Jokerst, D. R. Smith, and W. J. Padilla, “Design, theory, and measurement of a polarization insensitive absorber for terahertz imaging,” Phys. Rev. B, Vol. 79, No. 12, 125104, 2009.
9. Zhu, B., Z. Wang, C. Huang, Y. Feng, J. Zhao, and T. Jiang, “Polarization insensitive metamaterial absorber with wide incident angle,” Progress In Electromagnetics Research, Vol. 101, 231–239, 2010.
D. Shrekenhamer, N. I. Landy, K. Fan, X. Zhang, W. J. Padilla, and R. D. Averitt, “Highly flexible wide angle of incidence terahertz metamaterial absorber: Design, fabrication, and characterization,”Phys. Rev. B, Vol. 78, 241103 R, 2008.
11. Avitzour, Y., Y. A. Urzhumov, and G. Shvets, “Wide-angle infrared absorber based on a negative-index plasmonic metamaterial,” Phys. Rev. B, Vol. 79, No. 4, 045131, 2009. 12. Lagarkov, A. N., V. N. Kisel, and V. N. Semenenko,
“Wide-angle absorption by the use of a metamaterial plate,” Progress In Electromagnetics Research Letters, Vol. 1, 35–44, 2008.
13. Wen, Q. Y., H. W. Zhang, Y. S. Xie, Q. H. Yang, and Y. L. Liu, “Dual band terahertz metamaterial absorber: Design, fabrication, and characterization,”Appl. Phys. Lett., Vol. 95, No. 24, 241111, 2009.
14. Tao, H., C. M. Bingham, D. Pilon, K. Fan, A. C. Strikwerda, D. Shrekenhamer, W. J. Padilla, X. Zhang, and R. D. Averitt, “A dual band terahertz metamaterial absorber,” J. Phys. D: Appl. Phys., Vol. 43, 225102, 2010.
15. Mauskopf, P. D., J. J. Bock, H. Del Castillo, W. L. Holzapfel, and A. E. Lange, “Composite infrared bolometers with Si3N4 micromesh absorbers,”Appl. Opt., Vol. 36, No. 4, 765–771, 1997. 16. Parsons, A. D. and D. J. Pedder, “Thin-film infrared absorber structures for advanced thermal detectors,” J. Vac. Sci. Tech-nol. A, Vol. 6, No. 3, 1686–1689, 1988.
17. Rand, B. P., P. Peumans, and S. R. Forrest, “Long-range absorption enhancement in organic tandem thin-film solar cells containing silver nanoclusters,” J. Appl. Phys., Vol. 96, No. 12, 7519–7526, 2004.
18. Pillai, S., K. R. Catchpole, T. Trupke, and M. A. Green, “Surface plasmon enhanced silicon solar cells,” J. Appl. Phys., Vol. 101, No. 9, 093105, 2007.
19. Zhou, J. F., L. Zhang, G. Tuttle, T. Koschny, and C. M. Soukoulis, “Negative index materials using simple short wire pairs,” Phys. Rev. B, Vol. 73, No. 4, 041101, 2006.
20. Chen, X. D, T. M. Grzegorczyk, B. I. Wu, J. P. Jr, and J. A. Kong, “Robust method to retrieve the constitutive effective parameters of metamaterials,” Phys. Rev. E, Vol. 70, No. 1, 016608, 2004. 21. Reynolds, J. E, B. A. Munk, J. B. Pryor, and R. J. Marhefka,